### IOP Conference Series: Materials Science and Engineering

**PAPER • OPEN ACCESS**

### Techniques to accelerate thermo-mechanical simulations in large-scale

### FE models with nonlinear plasticity and cyclic input

**To cite this article: D Benasciutti et al 2019 IOP Conf. Ser.: Mater. Sci. Eng. 629 012008**

View the article online for updates and enhancements.

Content from this work may be used under the terms of theCreative Commons Attribution 3.0 licence. Any further distribution of this work must maintain attribution to the author(s) and the title of the work, journal citation and DOI.

Published under licence by IOP Publishing Ltd

The 2nd International Conference on Material Strength and Applied Mechanics
**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

1

**Techniques to accelerate thermo-mechanical simulations in **

**large-scale FE models with nonlinear plasticity and cyclic **

**input **

**D Benasciutti1,3 _{, F De Bona}2_{, L Moro}2_{ and J Srnec Novak}2**

1_{Department of Engineering, University of Ferrara, via Saragat 1, 44122 Ferrara, Italy }
2_{Politechnic Department of Engineering and Architecture (DPIA), University of }

Udine, via delle Scienze 208, 33100 Udine, Italy E-mail: [email protected]

**Abstract. A procedure is proposed to reduce the computation time of thermo-mechanical **

simulations with large nonlinear finite element (FE) models that involve cyclic plasticity. The procedure is helpful when it is practically unfeasible to simulate the huge amount of cycles needed to bring the material model to its fully stabilised state (an unfavourable situation that often occurs when small plastic strains are present), as required before assessing the structural durability. A “reference” test case, with combined kinematic and isotropic nonlinear model calibrated on actual material properties, is compared to accelerated models as well as pure kinematic models. Guidelines on how to set up the accelerated model are finally discussed.

**1. Introduction **

Structural durability of complex structures undergoing cyclic thermo-mechanical loadings may exploit results from elasto-plastic finite element (FE) analyses. On the one hand, the fatigue life assessment requires that the simulated cyclic material behavior reaches its complete stabilized condition (which occurs about at half the number of cycles to failure). On the other hand, attaining such a stabilized condition in large-scale nonlinear FE models may require that a huge number of cycles are simulated, which may become computationally unfeasible.

In a recent study dealing with elasto-plastic analysis of a copper mold for steelmaking plant [1], it was estimated that the three-dimensional FE model would had required thousands of cycles (around 60000) to simulate the material behavior until complete stabilization, due to the unfavorable combination of small plastic strains and low stabilization speed of the mold alloy. In turn, thousands of cycles would have last hundreds of simulation days, i.e. beyond any practical limit.

The use of accelerated material models, as proposed in [2], was considered a mean to keep the computation time within more acceptable limits. In accelerated models, the stabilization speed is increased up to a “fictitious” value (see figure 1), which permits the number of cycles for simulating the material behavior from the onset of plasticization up to the stabilized condition to be reduced considerably (and so the computation time, too). In some cases, however, the stabilization speed cannot be increased arbitrarily and unreasonably (figure 1) if one needs to prevent numerical converge issues or “unrealistic” results in simulations [2].

The 2nd International Conference on Material Strength and Applied Mechanics
**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

2

**Figure 1. Actual and accelerated model. Simulation time is **

*decreased if the stabilization speed b is increased from its actual *
value (A) to a “fictitious” value (B).

Checking the correctness of acceleration techniques is possible only by comparison with a “reference” case that permits the cyclic material behavior to be simulated until complete stabilization. In this work, the reference case is an axisymmetric FE model of a hollow copper mold subjected to cyclic thermal loadings.

**2. Plasticity model: Theoretical background **

The cyclic material behaviour is modelled through a combined kinematic and isotropic model [3]:

### (

### ) (

:### )

0 2 3 0 = − − − −

**X**

**S**

**X***R*

*(1)*

**S*** where S is the deviatoric stress tensor, X is the deviatoric back-stress tensor, R is the drag stress and σ*0

**is the initial yield stress. In the combined model, the yield surface both translates (controlled by X) and *** expands (controlled by R) as function of plastic strain increment dε*pl

*and accumulated plastic strain ε*pl,acc.

The kinematic part is based on the Chaboche’s nonlinear model [3]:

acc
pl,
i
i
pl
i
i
1
i
i d d
3
2
d
; *C* *ε*
*n*
**X****ε****X****X*** X*=

###

= − = (2)*where C is the hardening modulus and γ is the recovery parameter controlling the decay of C as plastic *
*strain accumulates. For i=1, equation (2) yields the Armstrong-Frederick model with only two pairs (C*1,
*γ*1* ). For γ=0, equation (2) gives the Prager model (linear kinematic), in which dX=(2/3)C*lin

*pl.*

**dε**The isotropic model, which controls the material hardening/softening, is based on the incremental
*relationship dR=b(R*∞*–R)dε*pl,acc*, in which R*∞* is the saturated stress and b is the stabilization speed for *

*hardening (R*∞*>0) or softening (R*∞<0). Integrating the previous expression gives [3]:

## (

## )

##

1 exp*b*

###

pl,acc##

*R*

*R*= _{} − − (3)

*The material stabilizes when R reaches R*∞, which (according to [3]) occurs approximately when the

*exponent bε*pl,acc*5. In strain-controlled fully reversed cycles characterized by a plastic strain range Δε*pl,

*the total plastic strain accumulated after N cycles is approximately 2NΔε*pl and the stabilized condition

*becomes 2bN*stab*Δε*pl*5 (where N*stab is the number of cycles to stabilization). This relationships shows

*that N*stab* is inversely proportional to both b and Δε*pl* (see figure 1) and explains why N*stab may become

really large in those situations in which plastic strain accumulates rather slowly, due to a material that
*has a small b and is subjected to cycles where plastic strain is not predominant. *

*Increasing b is but one of many techniques proposed in literature. If both creep and thermal fatigue *
are present, some authors [4,5] suggest that only a limited number of cycles can be simulated. Although
not well defined, this procedure could be justified by considering that visco-elasticity tends to reduce
the time to stabilization. If creep rupture constitutes the damage criterion in design, an extrapolation

**SIMULATION ERRORS**

**NOT FEASIBLE**
(computation time is too high)

*Cycles to stabilization, N*stab(log)
*(simulation time)*
Model
par
amet
er
(s
tabil
iz
ati
on
sp
ee
d,
*b*
)
actual model
accelerated
model
60000
*(630 days)*
100
*(25 hours)*
4
300
Δε_{pl}=cost A
B

The 2nd International Conference on Material Strength and Applied Mechanics
**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

3

technique aimed to speed up the simulation is proposed in [6]. In situations with no creep, other authors [7,8] adopt a kinematic model with stabilized material properties from the beginning of simulation (no isotropic model simulates the cyclic material hardening/softening).

**3. Numerical case study **

*3.1. Component description *

As benchmark, numerical simulations consider a mold for continuous casting of steel, which is a hollow
tube where the initial solidification of steel takes place (see figure 2(a)). The actual shape of mold cross
section (round, square, rectangular) depends on the shape of the final product. On its inner surface, the
*component is subjected to a massive thermal flux q that varies along its length, from a maximum q*max

(corresponding to the position of liquid steel) to a constant value. The overall thermal flux distribution also changes over time, from its full value (plant is in service) to zero (plant switched off). On its outer surface, the mold is water-cooled. The component is simply supported to the surrounding structure and is free to expand. Molds are made of copper alloys, as they have a favorable combination of high thermal conductivity and good mechanical strength. The mold analyzed in this study has length 1000 mm, inner diameter 200 mm and thickness 16 mm, and it is made of CuAg0.1 alloy, whose cyclic plasticity properties (estimated from experiments) are summarized in [9].

**Figure 2. (a) component; (b) axisymmetric finite element model and mesh zoom; **

(c) temperature distribution; (d) equivalent plastic strain distribution.

*3.2. Finite element model *

Thanks to the axial symmetry of geometry and boundary conditions, the mold can be represented by a two-dimensional (2D) axisymmetric FE model (see figure 2(b)), which moreover permits the computation time to be greatly reduced even when simulating hundreds of cycles. The model is constituted by 760 axisymmetric 8-node isoparametric elements, for a total of 2487 nodes. Mesh is refined in the region of maximum thermal flux (point A), where the highest temperatures and stress gradients are expected to occur. The mold thermo-mechanical response is simulated by a first thermal analysis that yields the temperature distribution, which is then input in following mechanical analysis.

*3.3. Thermal analysis results *

In thermal analysis, a thermal flux of 3.2 MW/m2_{ proposed in [10] is applied on the inner surface, a }

convection on the outer surface (with bulk temperature 40°C and convection coefficient 48000 W/m2_{K). }

**A**
*T*o_{C}
**A** **A**
(b) (c) (d)
a
r
ϴ
Critical point
A
D
is
ta
n
ce
f
ro
m
t
o
p
o
f
m
o
ld
Thermal Flux
(a)
axis of
axisymmetry

**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

4

The thermal flux from [10] was incremented by about 50% so that the maximum temperature reached the value 300°C for which material properties are available in [9]. The model also includes temperature dependent material properties. The change of heat flux is simulated by a sequence of steady-state analyses, are explained in [1].

Figure 2(c) displays the calculated temperature distribution. The largest temperature gradients are located close to the region of maximum thermal flux, where also the maximum temperature 298°C occurs at point A (this point will be monitored in structural analysis).

*3.4. Mechanical analysis results *

The input is the temperature field calculated in previous thermal analysis. No mechanical constraints are applied to the model, as the actual mold is free to expand. A nonlinear combined kinematic and isotropic material model is used and brought up to complete stabilization (“reference” case). Material parameter values are taken from [9] (the CuAg01 exhibits cyclic softening).

Results from the “reference” case were compared to those from other models, namely:

⚫ *accelerated (combined kinematic-isotropic) models, with an increased stabilization speed b*_{a}. In

order to make the sensitivity analysis the widest possible, eight values – covering a wider range
*than that suggested in [2] – were scrutinized (b*a*=0.01b, 10b, 20b, 30b, 100b, 200b, 300b, 421b); *
⚫ only kinematic model (linear) according to Prager;

⚫ only kinematic model (nonlinear), with the static parameters calibrated on either first or

stabilized cycle;

**Figure 3. Stress components vs. loading **

cycles.

** Figure 4. Evolution of hoop stress-strain at **

cycles (for clarity, only some cycles are plotted).
*For accelerated model, the value 0.01b represents a lower bound for which the contribution of *
isotropic part to the combined model becomes negligible (i.e. material does not show softening). By
*contrast, value 421b constitutes an upper bound for which cyclic softening occurs so rapidly that – as it *
will be discussed later on – unrealistic results (“distorted” stress-strain cycles) are obtained (for even
*higher b, simulation do not converge at all). For Prager and nonlinear kinematic models, the difference *
in material properties between initial state and stabilized state are considered by calibrating the elastic
*modulus and yield stress either on the first cycle (E*1, σ0*) or on the stabilized cycle (E*s, σ0*). Note that

the first quarter of first cycle corresponds to the monotonic uniaxial stress-strain curve.

The “reference” combined model takes about 537 cycles to make the material stabilize (adopting the stabilization criterion described in [11]), as also confirmed by the cyclic evolution of stress components (radial, hoop and axial stress), see figure 3. Figure 4 depicts the evolution of hoop stress-hoop strain cycles at certain intervals (for more clarity, not all cycles are shown). The change of shape thorough cycling is evident.

Figure 5 shows how, for various accelerated models, the maximum von Mises stress in each cycle

0 100 200 300 400 500
100
110
120
130
140
150
160
*N *
* *
(
MP
a)
_{,max}
_{a,max}
_{vM,max}

###

_{r,max}

### =0

**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

5

*changes over the applied cycles N (which are normalized to the cycles N*stab required to complete

stabilization, in order to better emphasize the various trends in the very first cycles). All models attain
*almost the same asymptotic stress value, except the model with b*a*=0.01b in which the isotropic model, *

is somehow “deactivated”. It follows that the material to exhibit any softening (the hardening shown is only due to the kinematic model and ends in the first 8 cycles).

**Figure 5. Evolution of max. von Mises stress **

over cycles for different accelerated models.

** Figure 6. Evolution of equivalent strain range **
over cycles for different accelerated models.
*Of more interest is to monitor the evolution of the equivalent strain range ∆ε*eq as defined in [12] (see

figure 6), as this parameter is used to assess the low-cycle fatigue life. For the “reference” model (not
*accelerated), the strain range ∆ε*eq increases throughout the whole loading cycles, with a maximum rise

of about 18%. This trend confirms that, if cyclic loading is stopped before material had reached complete
*stabilization and ∆ε*eq attained its asymptotic value, the fatigue life may be overestimated (in a

*Manson-Coffin curve, the life is indeed a nonlinear inverse function of strain range as ∆ε*eq–c*, where c is a material *

*parameter). Models with a stabilization speed only moderately increased (b*a*=10b÷30b) display a trend *

*similar to the “reference” case, whereas others with much higher values (b*a*=100b÷300b) follow a *

different behavior, in which stabilization is almost completed in the early cycles. In all models examined, though, the equivalent strain range never stays constant during cycles, which confirms how important is that, in simulations, the material reaches its stabilized state in order to avoid errors in following fatigue life assessment.

**Figure 7. Design diagram for T=300°C. *** Figure 8. Comparison of ∆ε*eq from all models.

*0.5N*stab
110
120
130
140
150
*N *
vM
,m
ax
(
MP
a)
*Reference (N*
stab=537)
*b*
a*=10b (N*stab=68)
*b*
a*=20b (N*stab=34)
*b*
a*=30b (N*stab=21)
*b*
a*=100b (N*stab=8)
*b*
a*=200b (N*stab=6)
*b*
a*=300b (N*stab=4)
*b*
a*=421b (N*stab=10)
*b*
a*=0.01b (N*stab=8)
1 *N*stab
*N*
*N *
vM
,m
ax
(
MP
a)
*Reference (N*
stab=537)
*b*
a*=10b (N*stab=68)
*b*
a*=20b (N*stab=34)
*b*
a*=30b (N*stab=21)
*b*
a*=100b (N*stab=8)
*b*
a*=200b (N*stab=6)
*b*
a*=300b (N*stab=4)
*b*
a*=421b (N*stab=10)
*b*
a*=0.01b (N*stab=8)
Lower bound
*(b*_{a}*=0.01b)*
*Upper bound (b*a*=421b)*
100 101 102
0.3
0.32
0.34
0.36
0.38
0.4
0.42
*N*_{stab}
eq
(
%
)
Reference
*b*_{a}*=10b*
*b*_{a}*=20b*
*b*
a*=30b*
*b*
a*=100b*
*b*_{a}*=200b*
*b*_{a}*=300b*
*b*_{a}*=421b*
*b*
a*=0.01b*
100 101 102
0.3
0.32
0.34
0.36
0.38
0.4
0.42
*N*_{stab}
eq
(%)
Reference
*b*_{a}*=10b*
*b*
a*=20b*
*b*
a*=30b*
*b*
a*=100b*
*b*
a*=200b*
*b*
a*=300b*
*b*
a*=421b*
*b*
a*=0.01b*
*Lower bound (b*a*=0.01b)*
*Upper bound (b*_{a}*=421b)*
100 101 102 103
0
500
1000
1500
2000
*N*
stab
*b *
Reference
*b*
a*=10b*
*b*
a*=20b*
*b*
a*=30b*
*b*
a*=100b*
*b*
a*=200b*
*b*
a*=300b*
*b*
a*=421b*
*b*
a*=0.01b*
64
.
0
eq
pl
eq, =
100 101 102 103
0
500
1000
1500
2000
*N*_{stab}
*b *
Reference
*b*
a*=10b*
*b*_{a}*=20b*
*b*_{a}*=30b*
*b*_{a}*=100b*
*b*_{a}*=200b*
*b*_{a}*=300b*
*b*_{a}*=421b*
*b*
a*=0.01b*
Lower bound
Upper bound
*Δε*pl,a-5=0.0587
*Δε*pl,θ-5=0.0759
*Δε*pl,r-5=0.1347
1 2 3 4 5 6 7 8 9 10 11
0.32
0.34
0.36
0.38
0.4
0.42
Material ID
eq
(
%
)
Reference
*b*_{a}*=10b*
*b*_{a}*=20b*
*b*_{a}*=30b*
*b*_{a}*=100b*
*b*_{a}*=200b*
*b*
a*=300b*
*b*
a*=421b*
*b*
a*=0.01b*
Non. Kin.-initial
Non. Kin.-stabilized
Prager
0 2 4 6 8 10 12 14
0.32
0.34
0.36
0.38
0.4
Case study
eq
(
%
)
Reference
*b*
a*=10b*
*b*
a*=20b*
*b*
a*=30b*
*b*
a*=100b*
*b*
a*=200b*
*b*
a*=300b*
*b*
a*=421b*
*b*
a*=0.01b*
Non. Kin.-initial
Non. Kin.-stabilized
Prager
Lower bound
Upper bound
Reference

**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

6

Figure 7 represents a sort of “design diagram” that applies the concepts sketched in figure 1. It
*correlates parameters b, N and ∆ε*pl* through the relationship 2bN*stab*Δε*pl5. The plastic strain range is

calculated at the 5th_{ simulated cycle. The three curves correspond to the three plastic strain range }

*components (∆ε*pl,a*=0.0554% axial, ∆ε*pl,θ*=0.0734% hoop, ∆ε*pl,r=0.1289% radial). Except for the two

*bound cases (b*a*=0.01 and b*a*=421b), the other points lie close to the analytical curves, whose validity is *

thus confirmed.

* Table 1. Number of cycles to stabilization and ∆ε*eq

*for point A (T=300°C).*

Material ID 1 2 3 4 5 6 7 8 9 10 11
Comb.
model
Accelerated models
NKIa _{NKS}b Prager
model
*10b * *20b * *30b * *100b * *200b * *300b * *421b * *0.01b *
*N*stab 537 68 34 21 8 6 4 10 8 8 10 5
*Δεeq *
(%)
0.400 0.402 0.402 0.402 0.400 0.401 0.398 0.397 0.339 0.339 0.366 0.357
*Δe *
(%)
0.41 0.40 0.36 -0.02 0.5 -0.48 -0.91 -15.30 -15.26 -8.60 -10.71

a_{ NKI – nonlinear kinematic model with initial parameters }
b_{ NKS - nonlinear kinematic model with stabilized parameters}

*Figure 8 compares the equivalent strain range ∆ε*eq in the stabilized state, from all the material models

*examined (pure kinematic models–both linear and nonlinear–are included, too). The values of ∆ε*eq

provide an indirect measure of structure durability, as they are inversely proportional to the low-cycle fatigue life in a Manson-Coffin diagram. Values from figure 8 are also listed in Table 1.

*Accelerated models yield comparable ∆ε*eq (with a maximum relative deviation of 0.5% from the

“reference” case), which in turn confirms that a moderate increase of the stabilization speed (below the
*upper bound b*a*=421b) would leave the estimated fatigue life unaltered if compared to the life estimated *

by the “reference” model. The upper bound value, of course, cannot be determined beforehand and needs be established for the specific engineering application under study.

*Of more interest is to observe how pure kinematic models always underestimate the ∆ε*eq of the

*“reference” case, with a maximum deviation up to 15%. The lowest ∆ε*eq comes from the nonlinear

*kinematic model considering “initial” state of material (E*1, σ0). Only a small improvement yet occurs if

the nonlinear kinematic model is calibrated based on static parameters obtained from the stabilized state, or it is replaced by the linear Prager model calibrated on the initial state.

Either way, it seems apparent that neglecting the isotropic part in the combined model does not seem very appropriate. One the one hand, using a linear kinematic model greatly simplifies the model calibration, as only the monotonic tensile curve is required without any cyclic experimental data. On the other hand, figure 8 confirms the conclusions in [2], which caution engineers about the use of pure kinematic models that – regardless of being calibrated on the initial or stabilized material state – do completely neglect the material hardening/softening and the corresponding change in elastic-plastic properties over cyclic loading.

**4. Guidelines for practical applications **

A test case is now briefly discussed to show how accelerated models can be applied in practice. For the
FE model in figure 2, the thermal flux from [10] is incremented by only 30%, so that the maximum
temperature is close to the value 250°C for which material parameters (and, in particular, the
*stabilization speed b) are available in [9]. *

*The relationship 2bN*stab*Δε*pl5 governs the set-up of the accelerated model. To be calibrated, that

*relationship needs the value of plastic strain range Δε*pl in one structure point. This value can be

*approximated by Δε*pl-5 after five cycles, which normally demands for a relatively short simulation time

*even with large-scale nonlinear FE models. The b parameter is known from experimental data. *

**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

7

*the corresponding simulation time). Therefore, after establishing a target value N**_{<N}

stab that yields a

*more affordable simulation time, the “fictitious” b*a*5/(2N***Δε*pl-5) for the accelerated model can be

*derived accordingly (for the example under study, N**_{=40 gives b}

a=200), see figure 9. Running 40 cycles

*with b*a* gives an equivalent strain range Δε*eq=0.3144%, which only deviates by 2.27% from the value

*obtained by simulating 1033 cycles with the actual b. This result then validates the procedure. *

**Figure 9. Design diagram for T=250°C [11]. ****5. Conclusions **

Selecting the most appropriate cyclic plasticity model is a crucial step in thermo-mechanical finite element analysis. It may happen that the material model that fits more closely the experimental cyclic plasticity behavior is also the one that, in finite element simulations, requires a too large number of cycles to reach its stabilized state. This would result in a very long computation time, especially with large-scale three-dimensional FE models.

This work implemented several plasticity models (combined kinematic and isotropic, accelerated, Prager and nonlinear kinematic with “initial” and “stabilized” parameters) and compared them in terms of the equivalent strain range. As a basis for comparison, a “reference” test case was considered, in which the plasticity model is fitted on actual experimental data and the simulation carried out until complete material stabilization. The comparison showed that pure kinematic models, even if calibrated on either the initial or stabilized material state, deviated from the “reference” equivalent strain range, thus overestimating the actual structure fatigue life. Pure kinematic models, neglecting the material hardening/softening, seem inadequate and their use not recommended. By contrast, accelerated kinematic-isotropic models were always closed to the “reference” case, if the stabilization speed is increased up to two orders of magnitude (which allows the computation time to be shortened significantly). Guidelines were finally provided on how, in practical numerical cases, the “increased” stabilization speed in accelerated models can properly be set up.

**References **

[1] *Srnec Novak J, Benasciutti D, De Bona F, Stanojević A and Huter P 2015 Procedia Engineering *

**133 688-97 **

[2] * Chaboche J L and Cailletaud G 1986 Comput. Struct. 23 23-31 *
[3]

**Chaboche J L 2008 Int. J. Plasticity 24 1642-93**[4] *Arya V K, Melis M E and Halford G R 1990 Finite Element Elastic-Plastic-Creep and Cyclic *

*Life Analysis of a Cowl Lip (NASA Technical Memorandum 102342) *

[5] *Amiable S, Chapuliot S, Constantinescu A and Fissolo A 2006 Fatigue Fract. Eng. Mater. Struct. *

**29 209-17 **

[6] **Kontermann C, Scholz A and Oechsner M 2014 Mater. High Temp. 31 334-42 ***N=40*
*Δε*pl,θ-5=0.0442
*Δε*pl,a-5=0.0327
*Δε*pl,r-5=0.0769
57
.
0
eq
pl
eq, =

**IOP Conf. Series: Materials Science and Engineering 629 (2019) 012008**

IOP Publishing doi:10.1088/1757-899X/629/1/012008

8

[7] **Li B, Reis L and de Freitas M 2006 Int. J. Fatigue 28 451-8 **

[8] **Campagnolo A, Berto F and Marangon C 2016 Theor. Appl. Fract. Mec. 81 76-88 **

[9] *Benasciutti D, Srnec Novak J, Moro L, De Bona F and Stanojević A 2018 Fatigue Fract. Eng. *

**Mater. Struct. 41 1364-77 **

*[10] Galdiz P, Palacios J and Thomas B G 2014 Proc. European Cont. Casting Conf. (Graz, Austria, *
June 23–26, 2014)

**[11] Srnec Novak J, De Bona F, Benasciutti D and Moro L 2018 MATEC Web of Conf. 165 19010 ***[12] Manson S S 1966 Thermal Stress and Low-cycle Fatigue (New York: McGraw-Hill) *